43D Woven FabricsPelin Gurkan UnalNamk Kemal University Department of Textile Engineering Turkey 1. IntroductionComposite material, also called composite, a solid material that results when two or more different substances, each with its own characteristics, are combined to create a new substance whose properties are superior to those of the original components in a specific application (Encyclopdia Britannica, 2011). Because the objective in manufacturing component is to produce a stiff and a strong material with a low density, these materials have found place in many application fields such as land transportation, marine, construction, aerospace and medical. There are two constituents in a composite material which are the reinforcement and matrix phases. From the matrix point of view, composites can be divided into three main categories; polymer, metal and ceramic matrix composites (Zhang, 2003). Based on the reinforcement mechanism, composites can be separated as particle reinforced (large particle, dispersion strengthened), fibre reinforced (continuous (aligned), and short fibres (aligned or random)) and structural composites (laminates, sandwich). Fibre reinforced composites have been first introduced in exterior parts of Corvette in 1953. Today, fibre reinforced composites are used in many application fields. Textile structural composites usually consist of stacked layers known as 2D laminates, exhibit better in-plane strength and stiffness properties compared to those of metals and ceramics (Bilisik, 2010, 2011; Mohamed&Bogdanovich, 2009). However, the application of 2D laminates in some critical structures in aircraft and automobiles has also been restricted by their inferior impact damage resistance and low through thickness mechanical properties when compared against the traditional aerospace and automotive materials such as aluminium alloys and steel (Mouritz et al., 1999). These structures have low out-of plane properties because of the lack of third direction reinforcements which will result in low delamination resistances (Chou, 1992). In order to improve interlaminar properties of the 2D laminates, three dimensional (3D) textile preforms have been developed by using different manufacturing techniques like weaving, knitting, braiding, stitching, and non-woven manufacturing. Among these manufacturing techniques, sewing and 3D weaving are the promising technologies which address the shortcomings of the stack-reinforced composites (Padaki et al., 2010). Since manufacturing technology has a direct effect on the fibre orientation and fibre volume fraction of the preform, the properties of the end product will vary depending on the production and end-use requirements (Peters, 1998). Although 3D woven preforms have been used for approximately forty years in different application fields, there is not a common understanding and definition of these fabrics
which make them difficult to comprehend. Therefore, this chapter attempts to make a detailed overview of 3D woven fabrics, basic structure of 3D woven fabrics, definitions and classifications of 3D woven fabrics in comparison with 2D woven fabrics.
2. Definition, classification and weave structures of 3D woven fabrics2.1 Definition of 3D woven fabrics A basic common definition of 3D fabric is that these types of fabrics have a third dimension in the thickness layer. In 3D-fabric structures, the thickness or Z-direction dimension is considerable relative to X and Y dimensions. Fibres or yarns are intertwined, interlaced or intermeshed in the X (longitudinal), Y (cross), and Z (vertical) directions (Badawi, 2007). 3D fabrics can also be defined as a single-fabric system, the constituent yarns of which are supposedly disposed in a three mutually perpendicular plane relationship (Behera&Mishra, 2008). According to Chen, structures that have substantial dimension in the thickness direction formed by layers of fabrics or yarns, generally termed as the three-dimensional (3D) fabrics (Chen, 2011). Although all textiles have a 3D internal structure, macroscopically most can be regarded as thin 2D sheets. By 3D fabrics, (1) thick multilayer fabrics in a simple regular form or (2) made in more complicated 3D shapes, (3) hollow multilayer fabrics containing voids and (4) thin 3D shells in complex shapes are meant (Hearle&Chen, 2009). Khokar defined 3D woven fabrics as a fabric, the constituent yarns of which are supposed to be disposed in a three-mutually-perpendicular-planes relationship (Khokar, 2001). 2.2 Classification of 3D woven fabrics When the classification of 3D woven fabrics are examined, it is observed that there are several classifications based on the shedding mechanisms, weaving process, geometries and configurations, interlacements and fibre axis according to the different researches (Khokar,1996 as cited in Soden&Hill, 1998; Chen, 2010; Soden&Hill, 1998;Bilisik, 2011). Khokar classified the 3D fabrics as follows (Khokar, 1996 as cited in Soden&Hill, 1998); 1. 2. The conventional 2D weaving process designed to interlace two orthogonal sets of threads (warp and weft). This produces an interlaced 2D fabric on a 2D weaving device. The conventional 2D weaving process designed to interlace two orthogonal sets of yarns (warp and weft) with an additional set of yarns functioning as binder warps or interlacer yarns in the through-the-thickness or Z direction. This is referred to as multilayer weaving and produces an interlaced 3D fabric constituting two sets of yarns on a 2D weaving device. The conventional 2D weaving process using three sets of yarns (ground warp, pile warp and pile weft) to produce pile fabrics, known as 2.5D fabrics. The conventional 2D weaving process using three sets of yarns to produce a noninterlaced fabric with yarns in the warp, weft and through-the-thickness directions. This produces a non-interlaced 3D fabric with three sets of yarns on a 2D weaving device. The 3D weaving process designed to interlace three orthogonal sets of yarns. The weaving shed operates both row-wise and column-wise. This produces a fully interlaced 3D fabric where all three sets of orthogonal yarns interlace on a specifically designed 3D weaving machine.
3D Woven Fabrics
A non-woven, non-interlaced 3D fabric forming process designed to connect three orthogonal sets of yarns together with no interlacing (weaving), interloping (knitting), or intertwining (braiding). The fabric is held together by a special binding process.
However Soden and Hill added a new category as 4A to Khokars classification for the fabrics that could be placed between categories 4 and 5 where the conventional 2D weaving process uses three sets of yarns to produce an interlaced 3D fabric with yarns in the warp, weft and through-the-thickness directions (Soden&Hill, 1998). Regardless of the types of machines used, weaving technology is capable of constructing 3D fabrics with many different geometrical shapes. Chen studied the configurations and geometries of the 3D woven fabrics and classified 3D woven fabrics into four different categories, as listed in Table 1 (Chen, 2007 as cited in Chen et al., 2011). Structure Solid Architecture Multilayer Orthogonal Angle Interlock Multilayer Single layer Multilayer Multilayer Orthogonal Angle Interlock Shape Compound structure, with regular or tapered geometry Uneven surfaces, even surfaces, and tunnels on different level in multi-directions Spherical shells and open box shells Tubular nodes and solid nodes
Hollow Shell Nodal
Table 1. 3D textile structures and weave architectures (Chen, 2011). 2.3 Weave structures and properties In 3D woven fabrics, generally multilayer, angle interlock and orthogonal weave architectures are the most widely used weave structures. While multilayer and angle interlock weave structures can be produced with conventional 2D weaving machines especially with shuttle looms, orthogonal weave architecture needs a special designed 3D weaving machine to be produced. Orthogonal weave structures consist of three sets of yarns that are perpendicular to each other (X, Y and Z coordinates). In this particular 3D woven fabric formation process, Z yarns interconnect all individual warp- and fill-directional yarns and thus solidify the fabric (Bogdanovich, 2007). Mechanical and structural properties of the composites having orthogonal weave architectures with various binding weaves and different numbers of layers were investigated (Chen&Zanini, 1997 as cited in Behera&Mishra, 2008). The results of the investigation are as follows: Since straight yarns exist in the orthogonal structures, tensile stiffness and strength properties of these structures are well regardless of type of binding weave. However, tensile stiffness and strength values of these weave structures are directly proportional with the number of layers.
Number of layers and binding weaves do not affect the breaking elongation of the orthogonal structures. This property is mostly dependent on the elongation properties of the yarns used. The shear rigidity and shearing hysteresis increases when more layers are involved. Tighter binding weaves and more layers of the orthogonal structure will produce higher bending stiffness and bending hysteresis.
Multilayer weave structures consist of multiple layers each of which have its own sets of warp and weft yarns. The connection of the layers is done by self-stitching (existing yarns) or central stitching (external sets of yarns). In angle interlock weave structures; there are at least two sets of yarns such as warp and weft. In some cases, in order to increase fibre volume fraction and in-plane strength, stuffer yarns can be ad